Mechanical and Flame-Retardant Properties of Nanocomposite Based on Epoxy Resin Combined with Epoxidized Linseed Oil, Which Has the Presence of Nanoclay and MWCNTs

One of the main disadvantages of epoxy resins is brittleness and flammability, which is one of the biggest threats and the reason for limiting advanced applications. In this study, Epikote 240 (EP) epoxy resin was plasticized with epoxidized flaxseed oil (ELO) at different concentrations (EP/ELO ratios 95/5; 90/10; 85/15; 80/20; 75/25). +en, nanoclay additives and MWCNTs are simultaneously dispersed into the EP/ELO blend by using ultrasonic vibration. +e dispersion of ELO and nanoclay additives (nanoclay and MWCNTs) in epoxy resin is observed by using the scanning electron microscope in combination with the XRD method. +e effect of ELO, nanoadditives on mechanical properties, and flame retardants is assessed by tensile strength, flexural strength, compressive strength, impact resistance, UL 94HBmethod, and limiting oxygen index. Experimental results have shown that the mixing ratio of 90/10 w/w is the ratio for good compatibility, high mechanical properties, and fire retardation compared with other ratios. When adding MWCNTs as well as nanoclay I.30E to Epikote 240 epoxy, the mechanical strength and fire resistance have changed greatly: tensile strength of 85.45MPa, flexural strength of 116.32MPa, compressive strength of 189.25MPa, impact resistance Izod of 24.37 kJ/m, and fire resistance reached at V1.


Introduction
Epoxy flaxseed oil is one of the biological polymers, and it is more advantageous compared with petroleum-based polymers, due to its eco-friendly nature and biodegradability. erefore, biopolymers are used to replace synthetic polymers derived from petroleum oil. e development of biodegradable polymers using "green materials" is important [1][2][3][4][5]. Vegetable oil is a valuable resource in the production of biodegradable polymers. Due to the low cost and environmental advantages of epoxidized vegetable oils, they have been synthesized for use as a new biodegradable polymer by many researchers [6][7][8][9]. Bisphenol F based epoxy resin (DGEBF) has been replaced by epoxyzed flaxseed oil with a content of 50% by weight, and 5% by weight of nanoclay was added [10]. e mixture including DGEBF and ELO was treated with methyl tetrahydrophthalic anhydride (MTHPA) as a curing agent and 1-methylimidazole as an accelerator. As a result, with the presence of ELO, the glasstransition temperature (Tg) of DGEBF decreased and decreased sharply when adding nanoclay. When using curing agents related to amine group, the Tg increased due to the limiting of the transition of the fractions caused by the borders between organic phase (amine) and inorganic phase (clay). Alam et al. reported the study on adding ELO into polylactic acid (PLA) with presence of MWCNTs to decrease Tg and improved the mechanical properties of materials. In this study, such various amounts of ELO as 5, 10, and 15% by weight were used and the decrease of Tg as well as the increase of the plasticity of PLA were proved. However, when adding MWCNTs, Tg of materials got slightly increased. It is caused by the adhesion and cross-links between MWCNTs and resin [10].
ELO and nanoclay were added into epoxy resin for the first time to improve the mechanical and retardant properties of materials which was reported by Das and Karak in 2009 with a study on retardant properties of epoxy/nanoclay nanocomposite based on vegetable oils. As a result, the tensile strength and hardness of materials were tripled. e limiting oxygen index (LOI) and UL 94 experiments proved that nanocomposite based on the vegetable oil Mesua ferrea L was be able to retard fire [11,12]. e above said data show that when adding ELO, which is a natural and eco-friendly oligomer, several properties of polymers were changed, for example, decrease in Tg and improvement in plasticity. However, studies on producing composite materials based on ELO with the presence of ELO are not enough, especially studies on fire-retardant properties and adding MWCNTs and nanoclay at the same time into epoxy resin. Nanoclay additives (nanoclay and MWCNTs) are also used simultaneously to enhance the mechanical and flame-retardant properties of nanocomposites based on epoxy [13,14]. However, at present, there have been no researches on manufacturing epoxy resin nanocomposites based on the synergies of three components: nanoclay, MWCNTs, and ELO. e goal of this work is to increase several mechanical properties of epoxy polymer material by mixing epoxidised linseed oil and epoxy resin and find the optimal mixing ratio. In this study, the flame retardants like antimony trioxide and chlorinated paraffins were combined with epoxy Epikote 240 resin/epoxidised linseed oil cured by diethylenetriamine (DETA) hardeners in order to increase the flammability and maintain the mechanical strength of this material. e combustion resistance and limiting oxygen index (LOI), UL 94 methods with transmission electron microscopy (FE-SEM), and XRD methods were used.
MWCNTs with a diameter of 40-45 nm and a length of around 3 μm were provided by Showa Denko Japan Co. Chlorinated paraffin-S52 (CPs) was purchased from China and contained a maximum of 52% of chlorine. Antimony oxide (ATO) was received from China as fine white powder, was melted at 656°C, and had a specific gravity of 5.7. Antimony trioxide is over than 99.0%, and the amount of antimony metal is approximately to be 83%. e average size of fine powder antimony trioxide was found to be 1.5 μm. Nanomer ® I.30E nanoclay (NanocorUSA) is a surfacemodified montmorillonite mineral which will disperse to nanoscale in epoxy resin systems. e dispersion creates a near-molecular blend commonly known as a nanocomposite. is new type of composite exhibits enhanced strength and thermal and barrier properties. I.30E is supplied as a white powder which disperses to particles so thin that they are nearly transparent in the resin matrix.

Preparation of Epoxy/Epoxidised Linseed Oil/MWCNTs/ Nanoclay
Mixture. Epoxy Epikote 240 resin was mixed with epoxidised linseed following other ratios (Table 1) in 250 ml round-bottomed three-neck flask, the mixture was stirred 1500 rounds/minute in 1 hour, and it had a thermal stability at 80°C. e homogeneous mixture was cured by DETA at the room temperature in 24 hours, and then it was dried at 80°C in 3 hours. After 7 days, the mixture was analyzed and mechanical properties were measured.

Analysis.
e curing level was determined by extracting with acetone in soxhlet in 24 hours. e Izod impact strength was determined according to the ASTM D265 standard in Tinius Olsen (USA) at a temperature 25°C and humidity 75%. e compressive strength was determined according to the ISO 178-1993 standard in INSTRON (USA) equipment with a crosshead speed 5 mm/min, temperature 25°C, and humidity 75%.
FE-SEM (Evacseq error codes, S-4800) was used to investigate the morphological effects of adding antimony trioxide and chlorinated paraffins to the epoxy resin. Every sample was sputter-coated with gold-palladium and placed under room vacuum to take FE-SEM images. e flame-retardant properties were tested by the limiting oxygen index (LOI) (Yasuda Seiki Seisakusho Ltd, Japan) according to JIS K720-1976, with sheet dimensions of 120 × 6.5 × 3.2 mm. e UL-94 rating was tested according to the UL-94 (ASTMD635-12) with sheet dimensions of 125 ± 5 mm long by 13.0 ± 0.5 mm wide and minimum thickness, 3.0 (− 0.0 + 0.2) mm. e combustion rate was measured by COMBUSTION RESISTANCE COD 6145000 according to the ASTM D757-77 standard. Specimen's dimensions were 3.17 × 12.7 × 121 mm 3 .
e mechanical properties were measured on an INSTRON-5582 100 KN (USA) according to ISO 527-1993 with an extension speed of 5 mm/min. All data were the average of five independent measurements; the relative errors committed on each data were reported as well. Table 1 shows that the level curing of the EP/ELO mixture decreased and time curing increased with increasing of ELO phr. e sample with the EP/ELO ratio is 20/80, had 3362 minutes of time curing, and 5.06% of level curing. For samples with EP/ELO ratio from 15/85, time curing was not identified, and after 7 days, the 100 ELO phr was not cured. Based on results of time curing and level curing, we chose the samples with EP/ELO ratios 95/5, 90/10, 85/15, 80/20, and 75/25 to study. Although the difference samples had suitable time curing, they were destroyed before measuring the mechanical properties because they had low mechanical properties. is showed that mixing ability and mechanical properties of materials decreased much when the content of ELO reached a limit.

Effects of Content of Epoxidised Linseed Oil on Mechanical
Properties of Epoxy Epikote 240 Polymer. Table 2 shows that the sample with EP/ELO ratio 90/10 had the highest mechanical strength with 88.7 MPa of flexural strength, 52.8 MPa of tensile strength, and 121.36 MPa of compressive strength. Compared with the initial epoxy polymer, the flexural strength increased by 2.24% and compressive strength lightly decreased because epoxidised linseed oil acted as a plasticized filler which improved the brittle property of the material.
When replacing partial synthetic polymers with different weights, the mechanical properties not only remain high compared with the synthetic polymers without mixing but also improve in some durability; in this case, the flexural strength increases, especially the Izod impact strength increases by 21.65%; this is a good result compared with the works being studied by Samper et al. [16,17]. us, when replacing a part of fossil-derived substances with substances of biological origin (ELO), gel time and mechanical strength are maintained at a good level [18] e impact of ELO content on the fire retardant property of EP/ELO materials is presented in Table 3. From Table 3, it is seen that the ELO content is more or less also affecting the flame-retardant property of the epoxy resin. When the content of ELO increases, the compatibility decreases, resulting in an unstable structure and causing the material fire retardation to decrease. Especially, the mixing ratio of 90/10 w/w is the ratio for good compatibility, high mechanical properties, and fire retardation compared to other ratios.

Investigation of Structure of Epoxy Epikote 240/Epoxidised
Linseed Oil. In Figure 1, the results showed that the sample with EP/ELO ratio 90/10 had a homogenous structure and did not have a splitting phase. When the content of ELO increased, the splitting phase appeared and ELO particles precipitated like the 80/20 sample that had ELO particles with nonuniform distribution and large size due to precipitation. e 90/10 sample with 20.000 times of resolution showed that the average size of ELO particles was 0.5 μm and they had uniform distribution and uniform size ( Figure 2). e surface of ELO particles was covered by epoxy resin substrate. In this study, the blending process between epoxy and ELO is carried out at room temperature without the use of compatible auxiliaries. e high level of compatibility is shown by the FE-SEM measurement, which is better than those studied at high temperatures and using a common catalyst methylhexahydrophthalic anhydride (MHHPA) [18,19].

Mechanical and Fire-Retardant Properties of Nanocomposite Materials Based on Epoxy Epikote 240 Combined with ELO with the Presence of Nanoclay I.30E, MWCNTs, and
Retardants. Samples were made according to the mass ratios in Table 4. Figure 3 shows the uniform distribution and good bonding of Sb 2 O 3 particles in epoxy resin. Evidences show that after break of materials, Sb 2 O 3 particles were still maintained in fracture surfaces and covered by epoxy E 240 resin (there was no space around the particles). MWCNTs were also distributed and interleaved with retardants (positioned by arrows). ere is no agglomerate and clustered      Figure 4 was quite nice. In Figure 5, FE-SEM image shows that MWCNTs and retardants were distributed uniformly in the epoxy background (positioned by arrows) as well as their good sticking and combination with epoxy resin E 240; the resin still covered Sb 2 O 3 and MWCNTs after breaking the samples by pulling. Figures 5 and 6 also prove the uniform distribution of nanoclay I.30E, MWCNTs, and retardants in epoxy resin E 240 as well as the good sticking between them. e XRD diagram of epoxy E 240-based nanocomposite materials is present in nanoclay, MWCNTs, and flame retardants, as shown in Figure 7. From Figure 7, nanoclay I.30E has been separated and alternated in epoxy E 240. For materials with flame-retardant surface, there are some peaks in the XRD diagram due to the composition of Sb 2 O 3 . e XRD pattern reveals that the organoclay gets delaminated in the epoxy matrix.
ELO and chlorinated paraffins make epoxy resin E 240 more flexible.
us, Table 5 shows that the impressive strength and tensile strength of samples decreased, but the flexural strength and impact strength strongly increased when ELO and chlorinated paraffins are added. A loose outer garment is worn over a swimsuit or exercise outfit. When adding MWCNTs and nanoclay I.30E into epoxy resin E 240, the mechanical strength was significantly changed. e decrease of the mechanical strength of materials when adding retardants was offset by advantages of MWCNTs and nanoclay I.30E.
In parallel with the above processes, MWCNTs were uniformly distributed in epoxy resin forming ash layers covering the material surface and preventing the contact between oxygen and the materials, limiting the development of flame. e ash layers uniformly spread in the material surface and made the samples not dripping when burning and improved the flame-retardant capability of epoxy resin. e combination of the flame-retardant mechanisms improved the flame-retardant capability of materials (Table 6). It can be said that the distribution ability of retardants in binders is more uniform, and the mechanical and retardant properties of materials improved. In this work, ELO has made E 240 epoxy resin more and more flexible, overcoming the brittle disadvantages of primary resins. Hence, the mechanical strength presented in Table 5 has shown that the compressive strength and tensile strength decrease slightly; however, the flexural strength and tensile strength increase at a high level. e assessment of fire resistance of nanocomposite materials ( Table 6) has shown that the level of fire resistance reaches V-1 for materials in the presence ELO. Obviously, the role of ELO is very important, which is a substance of biological origin to replace a part of fossil raw materials (epoxy resin), as it enhances the mechanical properties and flame-retardant properties to a good level compared with the prescribed standards. In addition, in this study, the material fabrication conditions were carried out under normal conditions and without the use of any other catalysts; the mechanical properties, flame-retardant properties, and compatibility are quite high compared with those of other studies [15,20,21]. e morphologies of residues after ignition by alcohol burner were investigated by SEM in Figure 8. It is worth noting that turning it into a char flake has a continuous surface under SEM in Figure8. is demonstrates that ELO has more or less impact on the

Conclusions
With this study, we can conclude that the nano/epoxy/ELO composites with different contents of ELO have been successfully modulated by mechanical methods and ultrasonic vibrations. XRD, FE-SEM, and studies on mechanical strength and fire resistance have confirmed the significant improvement in mechanical properties and fire resistance of nanocomposites. ELO can be used directly as a plasticizer to improve the flexibility, elasticity, and stability of heat-resistant polymers while being biodegradable and environment-friendly. ELO does not react with epoxide at room temperature; hence, ELO cannot be used in large amounts. ELO can only be added in small amounts (10% by weight) to increase the toughness. e appropriate optimal content of ELO in epoxy resin E 240 is 10% by weight of epoxy E 240   combination. UL94 and LOI tests showed a significant improvement in fire resistance of MWCNTs (0.02 wt.%)/ nanoclay (2 wt.%)/ELO (10 phr)/epoxy nanocomposite compared with pristine epoxy. So, the resulting system provides a potential high-performance material for many advanced applications.

Data Availability
e data used to support the findings of this study are available from the corresponding author upon request (https://anhnt@haui.edu.vn).

Conflicts of Interest
e authors declare that there are no conflicts of interest regarding the publication of this paper.